| ||Format||Pages||Price|| |
|PDF Version||6||$42.00||  ADD TO CART|
|Print Version||6||$42.00||  ADD TO CART|
Significance and Use
Test Method D6774, for determining maximum total contraction, crimp, and residual fiber shrinkage in textured filament yarns is suitable for acceptance testing of commercial shipments.
If there are differences of practical significance between reported test results for two laboratories (or more), comparative tests should be performed to determine if there is a statistical bias between them, using competent statistical assistance. As a minimum, use the samples for such a comparative tests that are as homogeneous as possible, drawn from the same lot of material as the samples that resulted in disparate results during initial testing and randomly assigned in equal numbers to each laboratory. The test results from the laboratories involved should be compared using a statistical test for unpaired data, a probability level chosen prior to the testing series. If a bias is found, either its cause must be found and corrected, or future test results for that material must be adjusted in consideration of the known bias.
The properties and their variability as measured by this method relate to bulk appearance, stretch and recovery of fabrics and dyeability of yarns.
For some yarns, elapsed time between processing and testing has a marked effect on the results, of this test, especially during the first 72 h. The effect is caused by stress decay which is known to be minimal beyond the seventh day and after which time the yarn remains relatively stable. Therefore, specimens should only be compared if tested after the same elapsed time. Samples can be tested at-line, thus having little to no elapsed time between processing and testing.
1.1 This test method covers the determination of crimp contraction, residual fiber shrinkage and their variability of all types of filament yarns (partially oriented yarn (POY), fully oriented yarn (FOY), flat yarns, textured and bulked continuous filament (BCF) carpet yarns) using an automated tester.
Note 1—For another method of testing crimp in textured yarns, refer to Test Method D4031.
1.1.1 This method may also be used for non-textured yarns.
1.2 This test method is limited to crimped, multi-filament yarns ranging from 22.0 to 890 dtex (15 to 800 denier) and for BCF yarns from 890 to 4200 dtex (800 to 3800 denier).
1.3 The values stated in either SI or US customary units are to be regarded separately as standard. Within the text, the U.S. customary units are in parentheses. The values stated in each system are not exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in nonconformance with the method.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D123 Terminology Relating to Textiles
D2258 Practice for Sampling Yarn for Testing
D4031 Test Method for Bulk Properties of Textured Yarns
D4849 Terminology Related to Yarns and Fibers
ICS Number Code 59.080.20 (Yarns)
UNSPSC Code 11151700(Yarns)